In this Chapter, we have shown that a nonlocal GL model Hamiltonian is capable of capturing the widely varying critical exponents for direct Mn-site doped per- ovskite manganite samples. The agreement of our present analytical estimates with experimental predictions indicates that the critical behavior near the PM-FM phase transition in such materials belong to the universality classes dictated by

4.5 Conclusion

the nonlocal GL model Hamiltonian [Eq. (4.1)]. Thus it signifies that the effec- tive interactions among the modes of the order parameter in these systems have a nonlocal character near the critical point. This is expected because these systems posses a strong spin-lattice coupling that gives rise to a nonlocal character to the interaction as discussed earlier.

In addition to its success in explaining the varying critical exponents in per- ovskite manganites and Mn-site doped manganese perovskites it appears that our nonlocal model might provide an opportunity to study the partially understood physics of systems in which high density of electrons are strongly coupled to lattice and, in particular, to elucidate the critical behavior of systems where competing interactions of several electronic and lattice degrees of freedom lead to extremely rich and complex physics.

**Chapter 5**

**Dynamic Critical Behavior of** **Perovskite Manganites**

**Summary**

We investigate the nonconserved critical dynamics of a nonlocal model Hamilto-
nian incorporating screened long-range interactions in the quartic term. Employ-
ing dynamic renormalization-group analysis at one-loop order, we calculate the
dynamic critical exponent *z* = 2 +*f*_{1}(*σ, w, n*) +*O*(^{2}) and the linewidth exponent

*$*=−*σ*+*f*_{2}(*σ, w, n*) +*O*(^{2}) in the leading order of , where= 4−*d*+ 2*σ*, with
*d* the space dimension, *n* the number of components in the order parameter, *σ*
and *w* are parameters coming from the nonlocal interaction term. The resulting
values of linewidth exponent*$*for a wide range of*σ*is found to be in good agree-
ment with the existing experimental estimates from spin relaxation measurements
in perovskite manganite samples.

**5.1** **Introduction**

The non-equilibrium dynamics of magnetic systems near the critical point received
a continual attention for decades[77,78,80,79,81,89,146]. In a typical scenario, the sys-
tem is quenched near the critical temperature*T*_{c} at time*t*= 0from an equilibrium
state away from *T*_{c}. A sudden quench near *T*_{c} causes the system to undergo a
slow relaxation towards the new equilibrium state, refereed to as the critical slow-
ing down. Theoretical models for the critical dynamics are usually based on a
Langevin-type equation governed by the Ginzburg-Landau (GL) Hamiltonian for
nonconserved or conserved order parameters[80,79,81,89,146]. These models eluci-
date the existence of various universality classes depending on the associated con-
servation laws and model parameters, namely, the number of components*n*of the
order parameter and the space dimensionality *d*. In addition to the two indepen-
dent static critical exponents [e.g., the correlation length exponent *ν* defined via
*ξ*∝ |*T* −*T*_{c}|^{−ν} and the Fisher exponent *η* for the algebraic decay of the two point
correlation function at criticality, *G*(**r**−**r**^{0})∝ |**r**−**r**^{0}|^{−(d−2+η)}], there exists a dy-
namic exponent *z* that governs the relaxation of the order parameter. The charac-
teristic time scale diverges as*τ*∝ |*T*−*T*_{c}|^{−zν} upon approaching the transition point
described as the the critical slowing down. Different values for *z* ensue depend-
ing on whether the order parameter is conserved and the existence of additional
conserved quantities. The simplest cases among them are the purely relaxational
models with either nonconserved (Model A) or conserved (Model B) order param-
eter Φ. The renormalization-group (RG) treatment for model A with short-range
(SR) interactions gives *z* = 2 +*cη* at two-loop order with *c*= 6 ln(^{4}_{3})−1, yielding
*z*= 1*.*984 in three dimensions^{[79,81,89]}.

While the above theoretical investigations were carried out for the model A with SR interactions, a long-range (LR) model was proposed by Fisher, Ma, and

5.1 Introduction

Nickel^{[57]} where the quadratic term in the model Hamiltonian was modified by
incorporating LR interactions. Following this (LR) model, the corresponding non-
conserved critical dynamics was investigated by Belim^{[19]}in a field theoretic frame-
work. Carrying out the calculations at two-loop order and employing the Padé-
Borel resummation technique, it was found that the LR interaction affects the
relaxation time of the system, indicated by the variation of *z* within the range
2*.*0000726*z*62*.*006628.

Recently, the perovskite manganites (R_{1−x}A_{x}MnO_{3}) have become the focus
of scientific and technological interest as they exhibit colossal magnetoresistance
(CMR)[148,68,14,197,42]. A number of experimental investigations on the critical
slowing down of such compounds near the paramagnetic-to-ferromagnetic (PM-
FM) phase transition were performed via a number of powerful techniques, namely,
muon spin relaxation (*µ*SR)^{[87,123]} spectroscopy, inelastic-neutron-scattering^{[230]},
pump-probe method^{[133,132]}, and magnetic resonance methods^{[13,253]}. In some of
these experiments^{[133,132]} the relaxation time exponent*νz* was measured for thin
film samples while in some other experiments[123,13,253], the linewidth exponent

*$*=*ν*(*z*+ 2−*d*−*η*)^{[79,90]} was measured for bulk samples. In Ref.^{[123]}, *µ*SR mea-
surements were performed on a single crystal of Nd_{0.5}Sr_{0.5}MnO_{3}exhibiting critical
slowing down of Mn ion spin fluctuations in the critical paramagnetic regime. This
facilitated the measurement of the linewidth exponent*$*from the relaxation of the
diffusive component, yielding *$*= 0*.*59±0*.*05. Using the electron-paramagnetic
resonance (EPR) technique, Atsarkin *et al.*^{[13]} investigated the critical slowing
down of longitudinal spin relaxation close to the PM-FM phase transition tem-
perature*T*_{c} in La_{1−x}Ca_{x}MnO_{3}for *x*= 0*.*2,0*.*25, and0*.*33. From the magnetic reso-
nance linewidth measurements, they obtained the linewidth exponent*$*≈0*.*5for
all samples. Using a similar experimental technique, Yassin*et al.*^{[253]}measured *$*

for La_{0.67−2x}Nd_{2x}Ca_{0.33−x}Sr_{x}MnO_{3} with *x*= 0, 0*.*1, 0*.*15, 0*.*2, and 0*.*25 and found

*$* to be nearly a constant (≈0*.*5) for all samples. These spin relaxation experi-
ments[123,13,253]indicate an interesting feature of perovskite manganite samples in
the sense that the linewidth exponent *$* near the critical point of PM-FM phase
transition is close to *$*≈0*.*5 independent of their chemical compositions (*x*, *R*,
and*A*).

The theoretical explanations for the magnetic (and electrical) properties of per-
ovskite manganites have so far been based on the framework of double exchange
(DE) interaction[255,148,197]and electron-phonon Jahn-Teller (JT) coupling^{[102,148]}.
However, as discussed in Ref.^{[13]}, the above mentioned experimental results (namely,
*w* ≈0*.*5) contradict the predictions of the polaron hopping model based on JT
lattice distortion, which was further confirmed in Ref.^{[253]}. It was in fact sug-
gested that the relaxation rate should increase near the critical temperature *T*_{c}
due to the formation of conduction band^{[201,202]}. Interestingly, Monte Carlo (MC)
simulations have been performed[32,158,157,156,54] on a model Hamiltonian in the
presence of DE interactions for the investigation of the static as well as dynamic
critical behavior. These simulations yield *ν*= 0*.*6949±0*.*0038, *β*= 0*.*3535±0*.*0030,
*γ*= 1*.*3909±0*.*0030in Ref.^{[32]},*β*≈0*.*365in Refs.^{[158,156]},*β*= 0*.*36±0*.*01in Ref.^{[157]},
and*ν*= 0*.*686±0*.*010,*β*= 0*.*356±0*.*006,*z*= 1*.*975±0*.*010in Ref.^{[54]}, which are close
to 3D Heisenberg model with SR interactions. This suggests that the DE and 3D
Heisenberg models^{[36,91]} belong to the same universality class.

In addition to the above investigations, a considerable number of experimen- tal studies have been conducted to find the static critical properties of doped per- ovskite manganite samples as elaborately discussed in Ch.3. These studies indicate the existence of diverse universality classes in such materials in the sense that they exhibit widely varying values of the static critical indices near the critical point by

5.1 Introduction

not only varying the doping level *x* but also by varying the sample composition
*R* and/or*A*. In contrast, as discussed above, experiments on the dynamic critical
behavior suggest an almost constant value for the linewidth exponent *$* (≈0*.*5)
although *x*, *R*, and *A* are varied in such samples. It can be guessed that such a
strange critical behaviour cannot follow from the DE model because it belongs to
the universality class of the SR Heisenberg model. Further, theoretical develop-
ments along the lines of the SR TDGL model^{[89]} and its modified LR version^{[19]}

cannot be expected to reproduce their widely varying critical indices. This neces- sitates an alternative model capable of capturing the static as well as the dynamic critical exponents observed for experimental samples.

The static critical behavior of a nonlocal model Hamiltonian was studied by
means of a Wilson type RG scheme in Ch. 3. The main distinguishing feature of
the non-local model Hamiltonian was the incorporation of the LR interactions in
the quartic term of the Ginzburg-Landau (GL) functional as^{R}*d*^{d}*x*^{R}*d*^{d}*x*^{0}Φ^{2}(**x**)*u*(**x**−
**x**^{0})Φ^{2}(**x**^{0}), where *u*(**x**−**x**^{0}) is a nonlocal screened coupling function. Quite satis-
factorily, this nonlocal model was found to represent a wide variety of universality
classes corresponding to the static critical behavior of a wide range of perovskite
manganite samples. This motivates us to investigate the dynamic critical behavior
governed by this nonlocal model Hamiltonian in the spirit of Model A of Halperin
and Hohenberg^{[80,89]}. Through this nonlocal model Hamiltonian, we are particu-
larly interested in capturing the dynamic critical behavior of perovskite manganites
near the PM-FM phase transition.

In this Chapter, we write the nonconserved Langevin dynamics for the order
parameterΦgoverned by the above mentioned nonlocal model Hamiltonian. Em-
ploying dynamic RG calculations at one-loop order we obtain the dynamic expo-
nent*z* and the linewidth exponent*$*in the leading order of, where= 4−*d*+ 2*σ*,

with*d*the space dimension and*σ*is a parameter occurring in the nonlocal interac-
tion term. Interestingly, the linewidth exponent *$* is found to be almost constant
(*$*≈0*.*5), although the static critical exponents vary with the nonlocal exponent*σ*
in the range−0*.*56*σ*60. The critical exponents agree well with the available ex-
perimental estimates for different samples. This suggests that the nonlocal model
Hamiltonian is a viable model for the critical behavior of PM-FM phase transition
in perovskite manganites.